called “fingering”, rather than a rapid, brittle fracture. Stringing can apply to both the diffusive bonding regime and the chemical bonding regime. The strings of molecules bridging across the gap would either be the molecules that had earlier diffused across the interface or the viscoelastic adhesive, provided that there was a significant volume of it at the interface. Microstructures The interplay of molecular scale mechanisms and hierarchical surface structures is known to result in high levels of static friction and bonding between pairs of surfaces. Technologically advanced adhesive devices sometimes make use of microstructures on surfaces, such as tightly packed periodic posts. These are biomimetic technologies inspired by the adhesive abilities of the feet of various arthropods and vertebrates (most notably, geckos). By intermixing periodic breaks into smooth, adhesive surfaces, the interface acquires valuable crack-arresting properties. Because crack initiation requires much greater stress than does crack propagation, surfaces like these are much harder to separate, as a new crack has to be restarted every time the next individual microstructure is reached. Hysteresis Hysteresis, in this case, refers to the restructuring of the adhesive interface over some period of time, with the result being that the work needed to separate two surfaces is greater than the work that was gained by bringing them together (W > γ1 + γ2). For the most part, this is a phenomenon associated with diffusive bonding. The more time is given for a pair of surfaces exhibiting diffusive bonding to restructure, the more diffusion will occur, the stronger the adhesion will become. The aforementioned reaction of certain polymer-on-polymer surfaces to ultraviolet radiation and oxygen gas is an instance of hysteresis, but it will also happen over time without those factors. In addition to being able to observe hysteresis by determining if W > γ1 + γ2 is true, one can also find evidence of it by performing “stop-start” measurements. In these experiments, two surfaces slide against one another continuously and occasionally stopped for some measured amount of time. Results from experiments on polymer-on-polymer surfaces show that if the stopping time is short enough, resumption of smooth sliding is easy. If, however, the stopping time exceeds some limit, there is an initial increase of resistance to motion, indicating that the stopping time was sufficient for the surfaces to restructure. Wettability and absorption Some atmospheric effects on the functionality of adhesive devices can be characterized by following the